Lime Treatment of Coal Bottom Ash for Use in Road Pavements: Application to El Jadida Zone in Morocco

Featured Application In this paper waste bottom ash from a thermal power station was treated with lime and sand. This improves certain material characteristics leading to a potential use in a subbase in road construction. Abstract Industrial waste causes environmental, economic, and social problems. In Morocco, the Jorf Lasfar Thermal Power Station produces two types of coal ash with enormous quantities: fly ash (FA) and Bottom ash (BA). FA is recovered in cement while BA is stored in landfills. To reduce the effects of BA disposal in landfills, several experimental studies have tested the possibility of their recovery in the road construction, especially as a subbase. In the first phase of this study, the BA underwent a physicochemical and geotechnical characterization. The results obtained show that the BA should be treated to improve its mechanical properties. The most commonly used materials are lime and cement. In the selected low-cost treatment, which is the subject of the second phase of the study, lime is used to improve the low pozzolanicity of BA while calcarenite sand is used to increase the compactness. Several mixtures containing BA, lime, and calcarenite sand were prepared. Each of these mixtures was compacted in modified Proctor molds and then subjected to a series of tests to study the following characteristics: compressive strength, dry and wet California Bearing Ratio (CBR), dry density and swelling. The composition of each mixture was based on an experimental design approach. The results show that the values of the compressive strength, the dry density, and the CBR index have increased after treatment, potentially leading to a valorization of the treated BA for use in a subbase.


Introduction
The fast expansion of infrastructure in developing countries, such as Morocco, increases the need for raw materials. In addition, the continued production of waste, in particular solid waste, requires the implementation of a waste storage system. This storage causes several economic, urban, and environmental problems. Therefore, there have been multiple studies over the possibility of using these by-products in the field of construction, including road construction [1,2]. In past years, different types of waste such as coal ash, steel slag and municipal solid waste incinerator ash [1,3,4] and other more recent waste types such as silicon waste [5] have been investigated in order to test the possibility of their valorization in civil engineering applications.

The Origin of the Materials
The BA is obtained from the JLEC plant EL Jadida, Morocco. They have been water-cooled and, therefore, they are recovered at the outlet of the boiler in a very humid (submerged) state, comparable to the moisture state of sea sand at the time of its extraction. Before being transported to the laboratory by truck (quantity necessary for all our tests), they were left outside the plant for three weeks in order to reduce their high water content sufficiently. Next, smaller quantities for each test batch were dried at the road geotechnical laboratory at the Hassania school of public works (Casablanca, Morocco).
To evaluate the pozzolanic reactivity of BA, mortar molds containing cement, sand, and water were prepared. Next, BA was used as a partial substitute for standardized sand. The compressive strength (CS) of the specimens containing the BA was compared with those of the conventional sand-based mortar. The cement used is the CPJ45 produced by the Holcim Lafarge Group in Morocco. Its chemical composition is given in Section 3.1.
As will be presented in the results, the BA has a porous structure, low compactness, and low pozzolanic reactivity. These weak characteristics do not allow for their use in a road foundation layer. To improve their performance, the BA was treated with lime and calcarenite sand. We note that the choice of these two treatment materials is made, taking into consideration the results of similar research [1]. They have proven the effectiveness of these two materials in improving the properties of BA. Lime is used to improve the pozzolanic activity of BA, while calcarenite sand increases its compactness. The lime used is produced at the Tetouan plant of the Lafarge group in Casablanca (Morocco). Its chemical composition is marked by a free lime (CaO) content greater than 80% whereas that of MgO does not exceed 8%. For the sand, we used a granular class 0/3.

Methodology
This work was carried out in three phases, summarized as follows: the first phase of this study consists of a complete characterization of the BA. The characterization tests cover density, chemical and mineralogical composition, cleanliness, granulometric analysis, Proctor test, and wet and dry CBR indices. The second part describes the experimental program including results obtained for the treatment of the BA using lime and sand. In this part, we also explain the experimental design, obtained by the Design-Expert software [18]. Lastly, the third phase of this study consists of the theoretical design of a pavement structure, with and without BA treated with lime and sand. The design is done according to the classical method of the 1998 new pavement type structure catalogue [19]. This method takes into consideration: traffic, climate and geotechnical environment of the El Jadida area in Morocco, which represents the location envisaged for the future pavement. The used methodology is shown in Figure 1. the laboratory by truck (quantity necessary for all our tests), they were left outside the plant for three weeks in order to reduce their high water content sufficiently. Next, smaller quantities for each test batch were dried at the road geotechnical laboratory at the Hassania school of public works (Casablanca, Morocco) .
To evaluate the pozzolanic reactivity of BA, mortar molds containing cement, sand, and water were prepared. Next, BA was used as a partial substitute for standardized sand. The compressive strength (CS) of the specimens containing the BA was compared with those of the conventional sand-based mortar. The cement used is the CPJ45 produced by the Holcim Lafarge Group in Morocco. Its chemical composition is given in section 3.1.
As will be presented in the results, the BA has a porous structure, low compactness, and low pozzolanic reactivity. These weak characteristics do not allow for their use in a road foundation layer. To improve their performance, the BA was treated with lime and calcarenite sand. We note that the choice of these two treatment materials is made, taking into consideration the results of similar research [1]. They have proven the effectiveness of these two materials in improving the properties of BA. Lime is used to improve the pozzolanic activity of BA, while calcarenite sand increases its compactness. The lime used is produced at the Tetouan plant of the Lafarge group in Casablanca (Morocco). Its chemical composition is marked by a free lime (CaO) content greater than 80% whereas that of MgO does not exceed 8%. For the sand, we used a granular class 0/3.

Methodology
This work was carried out in three phases, summarized as follows: the first phase of this study consists of a complete characterization of the BA. The characterization tests cover density, chemical and mineralogical composition, cleanliness, granulometric analysis, Proctor test, and wet and dry CBR indices. The second part describes the experimental program including results obtained for the treatment of the BA using lime and sand. In this part, we also explain the experimental design, obtained by the Design-Expert software [18]. Lastly, the third phase of this study consists of the theoretical design of a pavement structure, with and without BA treated with lime and sand. The design is done according to the classical method of the 1998 new pavement type structure catalogue [19]. This method takes into consideration: traffic, climate and geotechnical environment of the El Jadida area in Morocco, which represents the location envisaged for the future pavement. The used methodology is shown in Figure 1.

Characterization Methods
To test the possibility of using the BA in a foundation layer, several physicochemical and mechanical tests were carried out. The BA particles have a very porous shape. Their density is determined by the technique of the graduated cylinder [20], which consists in introducing a quantity of bottom ash in a known volume of water. The density is thus obtained by determining the volume occupied by this mass. The chemical composition of the BA Section 3.1 is obtained using X-ray fluorescence spectroscopy, while the mineralogical composition Section 3.1 is established using X-ray diffraction.
These two tests were carried out at the chemistry department at the Faculty of Sciences of the University of Hassan II in Casablanca, Morocco.
Next, the cleanliness of the BA is evaluated by two methods: sand equivalent (SE) method and methylene blue method according to the standards NF P18-598 [21] and NF P94-068 [22]. The first test gives us an idea of the rate of the clay part in our sample, the second determines the activity of this clay part and the degree of its sensitivity to water [23]. For the particle size analysis, the BA of class 0/20 mm was sieved according to the NF P18-560 standard [24], using 22 sieves from 0.04 up to 20 mm. The results obtained are compared to those specified by the ASTM standard [25] for BA used as a sand substitute [23]. In order to investigate the possibility of using BA in a road structure, the optimal compaction conditions, puncture resistance and swelling have been evaluated. In order to determine the optimal compaction conditions, the BA is sieved with a sieve of 20 mm and then subjected to a compaction test in a modified Proctor mold. The puncture resistance is measured twice: once compacted at natural water content as the dry CBR test (CBR d ) and then after immersion for four days, called the wet CBR or CBR after immersion (CBR w ). CBR d characterizes the ability of BA to withstand traffic flow. The swelling test is used to evaluate the behavior of BA under unfavorable humidity conditions. The swelling is measured during four days of immersion in order to test the volume stability of the BA [26]. The experimental protocols describing Proctor, CBR (dry and wet) and swelling test are detailed in the NF P94-078 standard [27].
Finally, the pozzolanic activity was judged. A material is pozzolanic if it can, in the presence of moisture, chemically react with calcium hydroxide to form compounds with binding properties. To evaluate the pozzolanic activity of BA, three series of mortar prisms of dimension 4 × 4 × 16 mm were prepared in the building materials laboratory of the Hassania School of Public Works (Casablanca, Morocco), see Figure 2a. The production procedure for mortars is described in the Moroccan standard NM 10.1.004 [20] for hydraulic binders. The first series is the standard mortar, containing 450 g of cement, 1350 g of standardized sand and 225 g of water, which gives three mortar prisms. In the second and third series, part of the normalized sand mass is replaced by BA of size 0/2 mm with percentages of respectively 25% and 50%. The prepared mixtures are introduced into the mortar molds, which will be stored in a wet cupboard at a temperature of 20 • C. After 24 h, they are demolded, then stored in a water bath at a constant temperature of 20 • C. The samples will be crushed after 7, 15, 28, 60, and 90 days to evaluate their compressive strength (CS).
Two different types of specimens were manufactured: • Figure 2a: mortar prisms (4 × 4 × 16) containing BA to study their pozzolanic activity (BA is used as a substitute for normalized sand); • Figure 2b: compacted test tubes of the BA specimens for the other characterization tests.

Overview of the Experimental Approach Adopted for the Treatment of BA
In order to improve the properties of the BA and with the intention of using them as foundation materials, they were subjected to a lime and sand treatment. The experimental approach adopted to establish mixing dosages and also to model the results is the design of experiments method [6]. The experimental design consists of selecting and ordering tests to identify the effects of parameters (factor Xi) on the desired properties (response Yi) of a material. These are statistical methods using simple mathematical concepts. The implementation of this method involves the following main steps: 1. Identification of the properties to be studied (responses); 2. Identification of the parameters (factors) that influence these responses; 3. Definition of the ranges of variation of each factor, with two levels of extreme variation (±1); 4. Carrying out the experiments planned by the model; 5. Analysis of the results (answers) and mathematical modeling.

Experimental Plan Adopted for the Treatment of BA
The final material studied is a mixture of BA treated with lime and sand. The factors considered to influence the properties of this mixture are: • The percentage of BA; • The water content noted as W; • The percentage of lime noted as L; • The percentage of calcarenite sand noted as S.
Other factors can be mentioned, such as the nature of the lime and sand, the compaction energy, the temperature during implementation, the mixing, and the storage conditions of the specimens. In this study, all of these were kept constant. In addition, the total solid mass of the mixture satisfies the following condition, given by Equation (1): The responses studied to evaluate the possibility of using the mixture as a foundation layer are: • Compressive strength at 60 days noted as CS60; • Dry density noted as γd; • Swelling noted as G; • Dry CBR index noted as CBRd; • The CBR index after immersion noted as CBRw.
There are several types of experimental design [18]. In this study, we opted for a centered composite factorial design composed of the following elements:  In order to improve the properties of the BA and with the intention of using them as foundation materials, they were subjected to a lime and sand treatment. The experimental approach adopted to establish mixing dosages and also to model the results is the design of experiments method [6]. The experimental design consists of selecting and ordering tests to identify the effects of parameters (factor X i ) on the desired properties (response Y i ) of a material. These are statistical methods using simple mathematical concepts. The implementation of this method involves the following main steps: 1.
Identification of the properties to be studied (responses); 2.
Identification of the parameters (factors) that influence these responses; 3.
Definition of the ranges of variation of each factor, with two levels of extreme variation (±1); 4.
Carrying out the experiments planned by the model; 5.
Analysis of the results (answers) and mathematical modeling.

Experimental Plan Adopted for the Treatment of BA
The final material studied is a mixture of BA treated with lime and sand. The factors considered to influence the properties of this mixture are: • The percentage of BA; • The water content noted as W; • The percentage of lime noted as L; • The percentage of calcarenite sand noted as S.
Other factors can be mentioned, such as the nature of the lime and sand, the compaction energy, the temperature during implementation, the mixing, and the storage conditions of the specimens. In this study, all of these were kept constant. In addition, the total solid mass of the mixture satisfies the following condition, given by Equation (1): The responses studied to evaluate the possibility of using the mixture as a foundation layer are: • Compressive strength at 60 days noted as CS 60 ; • Dry density noted as γ d ; • Swelling noted as G; The CBR index after immersion noted as CBR w .
There are several types of experimental design [18]. In this study, we opted for a centered composite factorial design composed of the following elements: An experimental point located in the center of the field of study; • Experimental points located on the axes of each of the 3 factors. These points belong to the interval (−α, +α).
The experimental design adopted will make it possible to evaluate the effects of the three factors at five different levels: −α, −1, 0, 1, and +α. The value of α is calculated as follows: α = NP 1/4 , with NP the number of points of the factorial plane. In our study this leads to the following value, Equation (2): The three main factors Lime (L), Water (W), and Sand (S) are associated with the reduced centered variables: A, B and C. The levels +α and −α are assigned to the extreme values of A, B and C. The levels −1, 0, and +1 are obtained by linear interpolation (see Table 1). The relationships between the reduced centered variables and the real variables are given by Equation (3)-(5): To obtain statistically representative results, each test is performed with three replicates. The number of specimens manufactured is distributed as follows: • 24 = 2 3 × 3 tests in the factorial design, in which the factors were adjusted to the −1 and +1 levels. In order to obtain results for CS 60 , γ d , G, CBR d and CBR w this study required (24 + 18 + 6) × 4 = 192 cylindrical specimens, see Figure 2b. All the tests are represented by the matrix included in Table 2. Table 2. Matrix of the tests of the composite centered factorial plan adopted for the treatment of bottom ash (BA).

Tests
Lime Dosage Water Dosage Sand Dosage

Chemical and Mineralogical Characteristics of Bottom Ash
The elemental composition of the studied BA and those found in the literature are given in Table 3. The results show that the BA mainly consists of silicon dioxide (SiO 2 ), aluminum oxide Al 2 O 3 and ferric oxide (Fe 2 O 3 ) with small amounts of calcium oxide, magnesium oxide, and potassium hydroxide. The sum of the percentages of the elements SiO 2 , Fe 2 O 3 , and Al 2 O 3 exceeds 80% of the total mass, while the percentage of CaO remains low. Therefore, BA can be classified as a silico-aluminous material (class F) according to the ASTM 225 standard [25]. This table also shows that the BA used in this study has a chemical composition that is very close to the BA found in literature [2,28,29]. In Table 1 of Reference [2] an overview is included showing the chemical analyses from different studies. The mineralogical composition of the BA, determined with X-Ray diffraction, reveals the existence of two peaks, see Figure 3. The first is quartz and the second is mullite. These two mineralogical phases are the same as those found for some BA studied in literature [28,29].
The mineralogical composition of the BA, determined with X-Ray diffraction, reveals the existence of two peaks, see Figure 3. The first is quartz and the second is mullite. These two mineralogical phases are the same as those found for some BA studied in literature [28,29].

Physical Characteristics of Bottom Ash
The visual observation of the BA shows that it has a gray color and a porous texture. Its absolute density is 1760 kg/m 3 . This value is low compared to natural aggregates such as silica sand which has an absolute density of 2600 kg/m 3 [28], and BA tested in [9] with an absolute density of 2560 kg/m 3 , but very close to the value for BA of 1880 kg/m 3 reported in [30]. In Table 2 from Reference [2] values ranging between 1390 and 2470 kg/m 3 are shown. The porous texture is the same as that observed for BA produced in other countries [2,28]. As discussed in Section 2.3, the cleanliness of the BA is verified by two tests: the sand equivalent (SE) and the methylene blue. The result of the first test is SE = 78%, which classifies the BA as clean sand with a low percentage of fine clay, which is ideal for construction work [19]. The second test yielded a methylene blue value of 0.5. This value is less than 1.5, which represents the threshold for silty sandy soils in sandy loam soils. It can be deduced from these two tests that the BA is clean and insensitive to water which encourages their use in the road domain.
The granulometric study of the BA (see Figure 4) shows that their particle size distribution (PSD) is very close to the sand. It also shows that their granulometric curve is located within the ASTM standard granular limits for BA used as foundation layer [31].

Physical Characteristics of Bottom Ash
The visual observation of the BA shows that it has a gray color and a porous texture. Its absolute density is 1760 kg/m 3 . This value is low compared to natural aggregates such as silica sand which has an absolute density of 2600 kg/m 3 [28], and BA tested in [9] with an absolute density of 2560 kg/m 3 , but very close to the value for BA of 1880 kg/m 3 reported in [30]. In Table 2 from Reference [2] values ranging between 1390 and 2470 kg/m 3 are shown. The porous texture is the same as that observed for BA produced in other countries [2,28]. As discussed in section 2.3, the cleanliness of the BA is verified by two tests: the sand equivalent (SE) and the methylene blue. The result of the first test is SE = 78%, which classifies the BA as clean sand with a low percentage of fine clay, which is ideal for construction work [19]. The second test yielded a methylene blue value of 0.5. This value is less than 1.5, which represents the threshold for silty sandy soils in sandy loam soils. It can be deduced from these two tests that the BA is clean and insensitive to water which encourages their use in the road domain.
The granulometric study of the BA (see Figure 4) shows that their particle size distribution (PSD) is very close to the sand. It also shows that their granulometric curve is located within the ASTM standard granular limits for BA used as foundation layer [31].

Compaction of Raw Bottom Ash
The Proctor test shows that the maximum density of the BA is 1.26 kN/m 3 , and is obtained at a water content of 21.6%. This high value of the Proctor moisture content indicates a high porosity of the material. Moreover, this value of the optimum Proctor of the BA is very low compared to

Compaction of Raw Bottom Ash
The Proctor test shows that the maximum density of the BA is 1.26 kN/m 3 , and is obtained at a water content of 21.6%. This high value of the Proctor moisture content indicates a high porosity of the material. Moreover, this value of the optimum Proctor of the BA is very low compared to conventional materials such as clay and sand whose dry density is respectively between 16 and 21 kN/m 3 . Hence the need to treat the BA in order to improve this characteristic.
The CBR d value obtained is 35%, exceeding the min. standard value of 20%. The BA is then classified in the lift class AR3 [26]. On the other hand, the punching test performed on a BA sample immersed for four days gives a CBR w value of 58%, which exceeds the CBR d value of 35%. This increase in lift is significant and should be exploited in the road sector.
Finally, the recorded value of the swelling (G) was zero. This result shows that the BA does not represent any risk of swelling and promotes its use in the road construction.

Pozzolanic Activity of BA
The evaluation of the mechanical behavior is performed by determining the compressive strength of mortar prisms, see Figure 2a, prepared from a mixture of CPJ 45 cement, water and BA as a partial substitute for the standardized sand. The results show that the compressive strength of the prisms containing BA is, at any age, adversely influenced by the use of BA, see Figure 5. The decrease in resistance becomes very important for 50% of BA and especially at a young age. These results are in the same order of magnitude as those found by other researchers [8,29]. They also found that the decrease of the compressive strength of mortar prisms containing BA can be explained by the dominant role of porosity, which is inversely proportional to compressive strength. In fact, the substitution of the most resistant material (standardized sand) by the weaker and more porous material (BA) increases the fraction of the pores of the mortar which decreases the compressive strength. a partial substitute for the standardized sand. The results show that the compressive strength of the prisms containing BA is, at any age, adversely influenced by the use of BA, see Figure 5. The decrease in resistance becomes very important for 50% of BA and especially at a young age. These results are in the same order of magnitude as those found by other researchers [8,29]. They also found that the decrease of the compressive strength of mortar prisms containing BA can be explained by the dominant role of porosity, which is inversely proportional to compressive strength.
In fact, the substitution of the most resistant material (standardized sand) by the weaker and more porous material (BA) increases the fraction of the pores of the mortar which decreases the compressive strength. As shown in Figure 5, an increase of the pozzolanic potential of the BA, especially at 60 and 90 days, becomes apparent. Therefore, during the treatment of the BA, the evolution of the compressive strength will be studied at 60 days instead of 28 days, because at this age the pozzolanic power of the BA is important and the compressive strength is significant. The composition of each mortar mixture and the values of their compressive strength at different ages (one sample per test) are given in Table 4.  As shown in Figure 5, an increase of the pozzolanic potential of the BA, especially at 60 and 90 days, becomes apparent. Therefore, during the treatment of the BA, the evolution of the compressive strength will be studied at 60 days instead of 28 days, because at this age the pozzolanic power of the BA is important and the compressive strength is significant. The composition of each mortar mixture and the values of their compressive strength at different ages (one sample per test) are given in Table 4. The average results and standard deviation of all tests performed on lime and sand treated BA are given in Table 5. Each value represents the average of three tests. These results show that in addition to the specific weight of the BA, mechanical properties such as compressive strength, and the dry and wet CBR indices are positively influenced by the addition of lime and sand. This result may be due to the increased compactness thanks to the addition of the sand or the activation of a pozzolanic reaction after the addition of lime. We also note that, for each treated BA mixture (TBA), CBR values after submersion (CBR w ) are higher than those of dry CBR (CBR d ) which represents a lift gain that cannot be found for conventional materials. This result is very interesting in terms of lift gain and reveals the importance of the use of BA in the road domain. Moreover, the swelling remains very low, as we wish, which encourages us to use the treated BA without risk of volume instability. The dry density was determined from its wet density using Equation (6):

Modeling Responses
For each response studied, we proceed to the modeling of the results using the Design-Expert software. This starts with the analysis of the variance, which allows the determination of the influencing factors and the elimination of the insignificant factors. Then a model combining each response to influential factors is developed. From this fact, a mathematical function connecting the response to the factors is proposed by the model. The modeling equations for the responses (CBR d , CBR w , γ d , G and CS 60 ) are expressed in terms of the percentages of lime (L), water (W) and sand (S). We thus obtain the following Equation (7)

Optimal Predicted Formulations
Taking into account the prerequisites of using BA as a foundation material, the models obtained make it possible for us to propose two optimal formulations, predicted from the actual test results.
The first optimal formulation is technical and takes into consideration the following requirements: 1.
Maximize CS 60 , CBR w , and CBR d .

2.
Minimize swelling (G) and percentages of lime and added sand.
The first optimal formulation is obtained with 2% of lime, 22.4% of water and 5% of sand. The predicted results for this first formulation are: The second variant is economical. It aims to reduce the cost by minimizing the processing materials while keeping acceptable mechanical properties and it takes into consideration the following requirements:
Minimize the cost 3.
CS60 > 1.5 MPa The second optimal formulation is obtained with 0.3% of lime, 22.4% of water and 20% of sand. The predicted results for the second formulation are: Both optimal formulations are acceptable although the compressive strength is less than 3 MPa. The CBR-values of both variants are sufficient for the proposed application and it is the major parameter taken into consideration for the dimensioning of this kind of structure. Moreover, the compressive strength parameter is studied in our case just to ensure the efficiency of the treatment. Higher compressive strength values are required for rigid structures (with concrete) which is not the case for our proposed pavement structure.

Use of Treated BA in Road Pavement
Characterization of the BA shows that they have very satisfactory characteristics: their granulometric curve is located inside the granular limits of BA valued in the roads. They are also clean and are insensitive to water. Moreover, their treatment with lime and sand has clearly improved their mechanical properties: compressive strength (CS 60 ), dry and wet CBR indices (CBR d , CBR w ) and dry density γ d all reached satisfactory levels after this treatment, while the swelling G remains very low. These results encourage us to use the BA in the foundation layer of a rural road, e.g. near the city of El Jadida in Morocco, thus minimizing transportation costs. The design method adopted is the classic method of the New Pavement Structure Catalog [19]. The parameters taken into consideration in the design of this route are the traffic which is class TPL3, the climate which is considered wet for the rural area of El Jadida, and the supporting ground which has a bearing capacity class of ST1. The conventional pavement structure proposed by the catalog, presented in Figure 6a, consists of 10 cm AC + 20 cm UGF2 + 20 cm UGB + SC, with: In the proposed pavement structure, we used the TBA (BA treated with lime and sand) as a foundation layer material instead of the UGF2. However, taking into account the modest CS of the TBA, we propose an increase in the thickness of the foundation layer, 30 cm of TBA instead of 20 cm of UGF2. The new proposed variant, see Figure 6b, consists of 10 cm AC + 30 cm TBA + 20 cm UGB + SC.

Conclusions
The results obtained in this study show that, despite their low density, the BA studied has interesting properties that can be used in order to promote their value in road engineering, particularly in the foundation layer. The results of this study are summarized as follows: 1. The Jorf Lasfar bottom ash BA is class F. It has a significant pozzolanic power, which favors their treatment with a hydraulic binder. 2. The lime treatment of the BA significantly improves their properties, which are: the compressive strength (CS60), the dry density, and the CBR indices. The best mechanical performances are obtained for a mixture with 4% of lime. 3. The use of calcarenite sand increases the dry density of the treated BA mixture (TBA) compared to that of the original BA. It is deduced that sand corrects the porous texture of BA by increasing their compactness. The maximum density is registered for 25% of sand. 4. According to the performance obtained after the treatment of BA with lime and sand, we propose their use as a road material in the rural roads of the city of El Jadida in Morocco. In the proposed pavement structure, we used the TBA as a foundation layer instead of the UGF2 (untreated granulate for foundation layer type 2). This valorization makes it possible, on the one hand, to provide a cheaper ecological rural road network and, on the other hand, to find a

Conclusions
The results obtained in this study show that, despite their low density, the BA studied has interesting properties that can be used in order to promote their value in road engineering, particularly in the foundation layer. The results of this study are summarized as follows: 1.
The Jorf Lasfar bottom ash BA is class F. It has a significant pozzolanic power, which favors their treatment with a hydraulic binder.

2.
The lime treatment of the BA significantly improves their properties, which are: the compressive strength (CS 60 ), the dry density, and the CBR indices. The best mechanical performances are obtained for a mixture with 4% of lime.

3.
The use of calcarenite sand increases the dry density of the treated BA mixture (TBA) compared to that of the original BA. It is deduced that sand corrects the porous texture of BA by increasing their compactness. The maximum density is registered for 25% of sand.

4.
According to the performance obtained after the treatment of BA with lime and sand, we propose their use as a road material in the rural roads of the city of El Jadida in Morocco. In the proposed pavement structure, we used the TBA as a foundation layer instead of the UGF2 (untreated granulate for foundation layer type 2). This valorization makes it possible, on the one hand, to provide a cheaper ecological rural road network and, on the other hand, to find a sustainable solution for landfilling the BA.
The results of this research constitute a first step forward in the field of valorization of BA in Moroccan pavements. However, the stakes remain very important if we take into account the millions of tons of this waste produced worldwide each year. Further research should include an analysis of leaching from the treated BA mixture and preferably a complete Life Cycle Assessment. If these studies are positive, the proposed pavement structure, containing BA, should be tested further, under real traffic conditions, in order to monitor its behavior and ensure its durability. Funding: This research was partly funded by the international office of the University of Antwerp and the VLIR-UOS South Programmes.